Presentation on theme: "Structural Engineering Lecture Series – September 22, 2007"— Presentation transcript:
1 Structural Engineering Lecture Series – September 22, 2007 Advanced Composite Material Applications in Structural Engineering Advances and ChallengesByAmjad J. ArefAssociate ProfessorStructural Engineering Lecture Series – September 22, 2007
2 OUTLINE Introduction: What are Composite Materials? Bridge ApplicationsFinal Remarks
3 What are Composite Materials? Composite structures are often called fiber reinforced polymer (FRP) structures, and polymer matrix composites (PMC).Composite materials are man-made, and must contain at least two constituents that are distinct chemically and physically.Intended to achieve an increase in certain properties such as stiffness, strength, fracture toughness among others, or decrease certain properties such as weight and corrosion. Composites in general can be categorized in two groups as follows:
5 ReinforcementLong continuous bundles l/d > 10 by definition, (typical dia for a fiber ~ 6-15 µm) unidirectional multidirectional woven or braided Continuous fibersShort chopped fibers randomly orientedWhiskers long thin crystals d< 1 micron length in the order of 100 microns used in ceramic matrix composites (CMC) and metal matrix composites (MMC)Particulates Near spherical not usually used for strength increase the toughness of the materialFlakes metallic, electrical/heating applications 2-D in nature, not usually used for strength
6 Reinforcement (cont’d) Glass (E-, S-, C-glass fibers) E-glass: Young’s modulus ~ 72 GPa, σu=3450 MPa (500 ksi ), Strain to failure 1-2%Carbon EL: GPa, ET=12-20 GPa σu= MPa ( ksi), strain to failure 0.5-1%Kevlar, Spectra (organic) E: GPa σu= MPa ( ksi), strain to failure 2-5%Ceramic fibers: high strength, stiffness and temperature stabilityAlumina (Al2O3) E: 370 GPa σu=1380 MPa (200 ksi)SiCBoron (toxic material), typically large diameter
9 Composites Categories Reinforced PlasticsLow strength and stiffnessInexpensiveGlass fibers is primary reinforcementApplications:Boat HullsCorrugated sheetsPipingAutomotive panelsSporting goodsAdvanced CompositesHigh strength and stiffnessExpensiveHigh performance reinforcement such as: graphite, aramid, kevlarApplications: Aerospace industry
10 Typical Applications in Structural Engineering Retrofitting of beams and columnsSeismic RetrofittingNew applicationsBridge DeckBridge Superstructure
11 FRP COMPOSITES IN STRUCTURAL APPLICATIONS AdvantagesHigh specific strength and stiffnessCorrosion resistanceTailored propertiesEnhanced fatigue lifeLightweightEase of installationLower life-cycle costsFactors preventing FRP from being widely acceptedHigh initial costsNo specificationsNo widely accepted structural components and systemsInsufficient data on long-term environmental durability
12 CONDITIONS OF U.S. HIGHWAY BRIDGES 28% of 590,000 public bridges are classified as “deficient”.The annual cost to improve bridge conditions is estimated to be $10.6 billion.Need for bridge systems thathave long-term durability andrequire less maintenance(Source: National Bridge Inventory)
13 Demand for FRP in Bridge Applications Is it necessary to use expensive FRP materials for bridge renewal?Given the massive investment to renew deficient bridges (28% of all bridges are deficient), repeating the same designs, materials, etc. may not be a prudent approach.Consider the fact that the average life span of a bridge in the U.S. is 42 years.FRP materials, if designed properly, could provide new bridges that last over 100 years.
14 GLASS FIBER REINFORCED POLYMER (GFRP) BOX SECTIONS The compressive flange is weaker than the tensile flange.A failure of a GFRP box section usually occurs in a catastrophic manner.The design of a GFRP box section is usually governed by stiffness instead of strength.Hybrid designorSpecial structuralsystem
15 BRIDGE APPLICATIONS – 1 (TOM’S CREEK BRIDGE) 203mm152 mmVirginia Tech and StrongwellPultruded composite beam (hybrid design of glass and carbon fibers and vinyl ester matrix)Span : 5.33 m , Width : 7.32 m
16 BRIDGE APPLICATIONS – 2 (TECH 21 BRIDGE) LJB Engineers & Architects, Inc. and Martin Marietta MaterialsLength : 10.1 m, Width : 7.3 mE-glass fiber reinforcement and polyester matrixDeck : pultruded trapezoidal tubes between two face sheets (tubes run parallel with the traffic direction)Stringer : three U-shaped structural beams838mm
17 BRIDGE APPLICATIONS – 3 (KINGS STORMWATER CHANNEL BRIDGE) UC San Diego, Alliant TechSystems, Inc., and Martin MariettaSpan: 2 x 10 m, Width: 13 mSix longitudinal concrete filled carbon tube girders (carbon/epoxy system)GFRP deck panel (pultruded trapezoidal E-glass/epoxy tubes with a top skin layerGFRP deckFilament wound CFRP tube
18 BRIDGE APPLICATIONS – 4 (TOOWOOMBA BRIDGE) University of Southern Queensland, Wagners Composite Fibre Technologies, and Huntsman CompositesSpan : 10 m, Width : 5.0 mHybrid box beams : prefabricated concrete, GFRP, and CFRP350450100(dimensions in mm)concreteGFRPCFRP
21 Recent Development of FRP Bridge Deck and Superstructure Systems
22 Hybrid-FRP-Concrete Bridge Deck and Superstructure System The system is developed at UB by an optimum selection of concrete and FRP.The system is validated analytically and experimentally to assess the feasibility of the proposed hybrid bridge superstructure and deck.Simple methods of analysis for the proposed hybrid bridge superstructure were developed.
23 BASIC CONCEPT OF PROPOSED HYBRID FRP-CONCRETE BRIDGE Single span with a span length of 18.3 mAASHTO LRFD Bridge SpecificationsLive load deflection checkdLL<L/800 under (1+IM)TruckService I limitDC+DW+Lane+(1+IM)TruckStrength I limit1.25DC+1.5DW+1.75[Lane+(1+IM)Truck]Concrete should fail first in flexure.A strength reduction factor for GFRP was taken as 0.4.18288 mm99mm1160mm3785 mmSimple-span one-lane hybrid bridge
24 PROPOSED HYBRID BRIDGE SUPERSTRUCTURE Advantages include:Increase in stiffnessCorrosion resistanceCost-effectivenessLightweightLocal deformation reductionHigh torsional rigidityPre-fabricationShort construction period
25 DISPLACEMENT AND STRENGTH CHECKS Deflection check: 0.61 x L/800Max. failure index : (safety factor=3.1)(a) Live load deflection check(b) Tsai-Hill Failure indexunder Strength I limit
26 TSAI-HILL FAILURE INDEX Failure condition :whereStrengths in the principal 1 and 2 directions and in-plane shearTensile and compressive directions
27 EXPERIMENTAL PROGRAM Materials Non-destructive tests Fatigue test GFRPConcreteNon-destructive testsFlexureOff-axis flexureFatigue testDestructive testsShearBearing
28 TEST SPECIMEN One-fifth scale model Span length = 3658 mm (dimensions in mm)
46 DESTRUCTIVE FLEXURE (TEST PROTOCOL) To examine the strength of the bridge and failure modesFlexural loadingDisplacement controlTwo stagesStep I (displacement history #1)Step II (displacement history #2)(a) Displacement history #1(b) Displacement history #2
47 DESTRUCTIVE FLEXURE (TEST RESULTS – 1) Failure load = 35 x Tandem loadlocalglobal
48 CHANGE OF A LOADING CONDITION From four point loads to two line loadscontact
49 DESTRUCTIVE FLEXURE (TEST RESULTS – 2) Failure modesConcrete crushingFailure of GFRP in compression
54 FINITE ELEMENT ANALYSIS ABAQUSFour-noded general shell element, S4R, for GFRP laminatesEight-noded general 3D solid element, C3D8, for concreteAssumed a perfect bonding between concrete and GFRPLinear analysisNonlinear analysis
55 FINITE ELEMENT DISCRITIZATION (LINEAR ANALYSIS) Number of nodes: 31,857Number of elements: 38,892 (22,764 for S4R and 16,128 for C3D8)
56 LINEAR FEA RESULTS (FLEXURE – 1) Stiffness was predicted by FEA within 5% error.
57 LINEAR FEA RESULTS (FLEXURE – 2) (a) Top surface(b) Bottom surface
58 LINEAR FEA RESULTS (FLEXURE – 3) Bottom surfacealong the center-line(b) Exterior web over height
59 FINITE ELEMENT DISCRETIZATION (NONLINEAR ANALYSIS) A quarter modelxyLoadingpoint
62 SIMPLE METHODS OF ANALYSIS Beam analysisOrthotropic plate analysisClassical lamination theoryUse of effective engineering properties of laminatesPerfect bonding between concrete and GFRP was assumed.Shear deformation was neglectedPrimary objective is to obtain deflection under design loads.
63 BEAM ANALYSISThe bridge is modeled as a beam with a span length, L, effective flexural rigidity, EIeff, and effective torsional rigidity, GJeff.whereEffective modulusEffective shear modulusVertical coord. from the neutral axisArea enclosed by median lines of the top and bot. flanges and exterior websAxis along the median line of a component
64 ORTHOTROPIC PLATE ANALYSIS The bridge is modeled as an orthotropic plate with span length of L and width of W.whereVertical displacementDistributed load on the plateRigidities that can be obtained by using the classical lamination theory
65 REPRESENTATIVE UNITS FOR THE PLATE ANALYSIS (a) Longitudinal direction(b) Transverse direction
66 SIMPLE METHODS OF ANALYSIS (UNDER TANDEM LOAD ONLY) (a) Transverse direction(b) Longitudinal direction
67 SummaryComposite materials hold great promise for effective renewal of deficient bridges.The hybrid FRP-concrete bridge superstructure is highly feasible from the structural engineering point of view.GFRP used in this study has revealed that its stress-strain relationship is not perfectly linear-elastic. However, for design purposes, the equivalent linear model can be used.
68 Summary (CONT’D)As is often the case with all-composite bridges, the design of the hybrid bridge superstructure is also stiffness driven.Results from a series of quasi-static tests have shown an excellent performance of the proposed hybrid bridge under live loads.The beam and orthotropic plate simplified analyses have proven to be effective to accurately predict the deflection of the hybrid bridge under design loads.
69 ChallengesA systematic way to determine design parameters should be developed. It is also important to propose and optimize the design based on life-cycle cost as well as performance.Long-term performance of FRP bridges is not yet established and should be investigated:creep, fatigue, and material degradation.Thermal effects on FRP bridges is still unknown and should be investigated.Quality control concerns— the material properties are highly dependent on the manufacturing process.
70 Challenges (CONT’D)Several practical aspects of FRP applications in bridges need to be addressed by researchers. The following are some of the outstanding issues:Methods to expand lanesMethods to cast concreteConsiderations for negative momentsConcrete barrier or steel parapetSupport conditions
71 Challenges (CONT’D)There are benefits in using light FRP deck or superstructure in bridges located in moderate and seismic regions.Automated fabrication process must be used to fabricate the FRP parts of the superstructure or deck.
72 AUTOMATED FABRICATION PROCESSES PultrusionRTMVARTMUse of braided fabricsFilament Winding
73 Acknowledgment Dr. Y. Kitane Dr. W. Alnahhal New York State Department of Transportation
Your consent to our cookies if you continue to use this website.